The material structure described by LiCrP3H8O13 crystallizes in the triclinic P-1 space group. There are two inequivalent Li sites. In the first Li site, Li(1) is bonded to two equivalent O(2), two equivalent O(5), and two equivalent O(6) atoms to form LiO6 octahedra that share corners with two equivalent P(1)O4 tetrahedra and edges with two equivalent Cr(1)O7 pentagonal bipyramids. In the second Li site, Li(2) is bonded to two equivalent O(10), two equivalent O(7), and two equivalent O(9) atoms to form LiO6 octahedra that share corners with two equivalent P(2)O4 tetrahedra, corners with two equivalent P(3)O4 tetrahedra, and edges with two equivalent Cr(1)O7 pentagonal bipyramids. Cr(1) is bonded to one O(1), one O(10), one O(2), one O(3), one O(5), one O(8), and one O(9) atom to form distorted CrO7 pentagonal bipyramids that share  a cornercorner with one P(3)O4 tetrahedra, corners with two equivalent P(1)O4 tetrahedra, corners with two equivalent P(2)O4 tetrahedra,  an edgeedge with one Li(1)O6 octahedra, and  an edgeedge with one Li(2)O6 octahedra. There are three inequivalent P sites. In the first P site, P(1) is bonded to one O(1), one O(12), one O(4), and one O(5) atom to form PO4 tetrahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent Cr(1)O7 pentagonal bipyramids,  a cornercorner with one P(2)O4 tetrahedra, and  a cornercorner with one P(3)O4 tetrahedra. The corner-sharing octahedral tilt angles are 56°. In the second P site, P(2) is bonded to one O(10), one O(11), one O(3), and one O(4) atom to form PO4 tetrahedra that share  a cornercorner with one Li(2)O6 octahedra, corners with two equivalent Cr(1)O7 pentagonal bipyramids,  a cornercorner with one P(1)O4 tetrahedra, and  a cornercorner with one P(3)O4 tetrahedra. The corner-sharing octahedral tilt angles are 54°. In the third P site, P(3) is bonded to one O(11), one O(12), one O(13), and one O(9) atom to form PO4 tetrahedra that share  a cornercorner with one Li(2)O6 octahedra,  a cornercorner with one Cr(1)O7 pentagonal bipyramid,  a cornercorner with one P(1)O4 tetrahedra, and  a cornercorner with one P(2)O4 tetrahedra. The corner-sharing octahedral tilt angles are 53°. There are eight inequivalent H sites. In the first H site, H(1) is bonded in a single-bond geometry to one O(2) atom. In the second H site, H(2) is bonded in a single-bond geometry to one O(7) atom. In the third H site, H(3) is bonded in a distorted single-bond geometry to one O(13) and one O(2) atom. In the fourth H site, H(4) is bonded in a single-bond geometry to one O(6) atom. In the fifth H site, H(5) is bonded in a single-bond geometry to one O(7) atom. In the sixth H site, H(6) is bonded in a distorted single-bond geometry to one O(6) and one O(8) atom. In the seventh H site, H(7) is bonded in a single-bond geometry to one O(8) atom. In the eighth H site, H(8) is bonded in a single-bond geometry to one O(6) atom. There are thirteen inequivalent O sites. In the first O site, O(1) is bonded in a distorted bent 150 degrees geometry to one Cr(1) and one P(1) atom. In the second O site, O(2) is bonded in a distorted water-like geometry to one Li(1), one Cr(1), one H(1), and one H(3) atom. In the third O site, O(3) is bonded in a linear geometry to one Cr(1) and one P(2) atom. In the fourth O site, O(4) is bonded in a bent 120 degrees geometry to one P(1) and one P(2) atom. In the fifth O site, O(5) is bonded in a 3-coordinate geometry to one Li(1), one Cr(1), and one P(1) atom. In the sixth O site, O(6) is bonded in a distorted water-like geometry to one Li(1), one H(4), one H(6), and one H(8) atom. In the seventh O site, O(7) is bonded in a distorted water-like geometry to one Li(2), one H(2), and one H(5) atom. In the eighth O site, O(8) is bonded in a distorted water-like geometry to one Cr(1), one H(6), and one H(7) atom. In the ninth O site, O(9) is bonded in a distorted trigonal planar geometry to one Li(2), one Cr(1), and one P(3) atom. In the tenth O site, O(10) is bonded in a 2-coordinate geometry to one Li(2), one Cr(1), and one P(2) atom. In the eleventh O site, O(11) is bonded in a bent 120 degrees geometry to one P(2) and one P(3) atom. In the twelfth O site, O(12) is bonded in a bent 120 degrees geometry to one P(1) and one P(3) atom. In the thirteenth O site, O(13) is bonded in a 2-coordinate geometry to one P(3) and one H(3) atom. is represented by the CIF card [CIF]
data_LiCrP3H8O13
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   7.185
_cell_length_b   7.693
_cell_length_c   9.965
_cell_angle_alpha   82.722
_cell_angle_beta   74.424
_cell_angle_gamma   77.856
_symmetry_Int_Tables_number   1
_cell_volume   517.249
_cell_formula_units_Z   2
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.000  0.000  0.000  1.0
  Li  Li1  1  0.000  0.500  0.500  1.0
  Cr  Cr2  1  0.807  0.819  0.770  1.0
  Cr  Cr3  1  0.193  0.181  0.230  1.0
  P  P4  1  0.326  0.805  0.742  1.0
  P  P5  1  0.242  0.806  0.475  1.0
  P  P6  1  0.593  0.459  0.731  1.0
  P  P7  1  0.407  0.541  0.269  1.0
  P  P8  1  0.758  0.194  0.525  1.0
  P  P9  1  0.674  0.195  0.258  1.0
  H  H10  1  0.360  0.980  0.964  1.0
  H  H11  1  0.819  0.817  0.430  1.0
  H  H12  1  0.311  0.862  0.101  1.0
  H  H13  1  0.920  0.739  0.205  1.0
  H  H14  1  0.691  0.694  0.398  1.0
  H  H15  1  0.858  0.665  0.009  1.0
  H  H16  1  0.651  0.628  0.001  1.0
  H  H17  1  0.099  0.660  0.086  1.0
  H  H18  1  0.901  0.340  0.914  1.0
  H  H19  1  0.349  0.372  0.999  1.0
  H  H20  1  0.142  0.335  0.991  1.0
  H  H21  1  0.309  0.306  0.602  1.0
  H  H22  1  0.080  0.261  0.795  1.0
  H  H23  1  0.689  0.138  0.899  1.0
  H  H24  1  0.181  0.183  0.570  1.0
  H  H25  1  0.640  0.020  0.036  1.0
  O  O26  1  0.474  0.877  0.791  1.0
  O  O27  1  0.270  0.983  0.058  1.0
  O  O28  1  0.193  0.965  0.379  1.0
  O  O29  1  0.361  0.863  0.575  1.0
  O  O30  1  0.112  0.854  0.813  1.0
  O  O31  1  0.974  0.745  0.101  1.0
  O  O32  1  0.826  0.715  0.379  1.0
  O  O33  1  0.788  0.630  0.943  1.0
  O  O34  1  0.758  0.560  0.672  1.0
  O  O35  1  0.083  0.710  0.559  1.0
  O  O36  1  0.422  0.661  0.389  1.0
  O  O37  1  0.381  0.589  0.746  1.0
  O  O38  1  0.417  0.653  0.134  1.0
  O  O39  1  0.583  0.347  0.866  1.0
  O  O40  1  0.619  0.411  0.254  1.0
  O  O41  1  0.578  0.339  0.611  1.0
  O  O42  1  0.917  0.290  0.441  1.0
  O  O43  1  0.242  0.440  0.328  1.0
  O  O44  1  0.212  0.370  0.057  1.0
  O  O45  1  0.174  0.285  0.621  1.0
  O  O46  1  0.026  0.255  0.899  1.0
  O  O47  1  0.888  0.146  0.187  1.0
  O  O48  1  0.639  0.137  0.425  1.0
  O  O49  1  0.807  0.035  0.621  1.0
  O  O50  1  0.730  0.017  0.942  1.0
  O  O51  1  0.526  0.123  0.209  1.0
[/CIF]
.
The material structure described by LiCrP3H8O13 crystallizes in the triclinic P-1 space group. There are two inequivalent Li sites. In the first Li site, Li(1) is bonded to two equivalent O(2), two equivalent O(5), and two equivalent O(6) atoms to form LiO6 octahedra that share corners with two equivalent P(1)O4 tetrahedra and edges with two equivalent Cr(1)O7 pentagonal bipyramids. In the second Li site, Li(2) is bonded to two equivalent O(10), two equivalent O(7), and two equivalent O(9) atoms to form LiO6 octahedra that share corners with two equivalent P(2)O4 tetrahedra, corners with two equivalent P(3)O4 tetrahedra, and edges with two equivalent Cr(1)O7 pentagonal bipyramids. Cr(1) is bonded to one O(1), one O(10), one O(2), one O(3), one O(5), one O(8), and one O(9) atom to form distorted CrO7 pentagonal bipyramids that share  a cornercorner with one P(3)O4 tetrahedra, corners with two equivalent P(1)O4 tetrahedra, corners with two equivalent P(2)O4 tetrahedra,  an edgeedge with one Li(1)O6 octahedra, and  an edgeedge with one Li(2)O6 octahedra. There are three inequivalent P sites. In the first P site, P(1) is bonded to one O(1), one O(12), one O(4), and one O(5) atom to form PO4 tetrahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent Cr(1)O7 pentagonal bipyramids,  a cornercorner with one P(2)O4 tetrahedra, and  a cornercorner with one P(3)O4 tetrahedra. The corner-sharing octahedral tilt angles are 56°. In the second P site, P(2) is bonded to one O(10), one O(11), one O(3), and one O(4) atom to form PO4 tetrahedra that share  a cornercorner with one Li(2)O6 octahedra, corners with two equivalent Cr(1)O7 pentagonal bipyramids,  a cornercorner with one P(1)O4 tetrahedra, and  a cornercorner with one P(3)O4 tetrahedra. The corner-sharing octahedral tilt angles are 54°. In the third P site, P(3) is bonded to one O(11), one O(12), one O(13), and one O(9) atom to form PO4 tetrahedra that share  a cornercorner with one Li(2)O6 octahedra,  a cornercorner with one Cr(1)O7 pentagonal bipyramid,  a cornercorner with one P(1)O4 tetrahedra, and  a cornercorner with one P(2)O4 tetrahedra. The corner-sharing octahedral tilt angles are 53°. There are eight inequivalent H sites. In the first H site, H(1) is bonded in a single-bond geometry to one O(2) atom. In the second H site, H(2) is bonded in a single-bond geometry to one O(7) atom. In the third H site, H(3) is bonded in a distorted single-bond geometry to one O(13) and one O(2) atom. In the fourth H site, H(4) is bonded in a single-bond geometry to one O(6) atom. In the fifth H site, H(5) is bonded in a single-bond geometry to one O(7) atom. In the sixth H site, H(6) is bonded in a distorted single-bond geometry to one O(6) and one O(8) atom. In the seventh H site, H(7) is bonded in a single-bond geometry to one O(8) atom. In the eighth H site, H(8) is bonded in a single-bond geometry to one O(6) atom. There are thirteen inequivalent O sites. In the first O site, O(1) is bonded in a distorted bent 150 degrees geometry to one Cr(1) and one P(1) atom. In the second O site, O(2) is bonded in a distorted water-like geometry to one Li(1), one Cr(1), one H(1), and one H(3) atom. In the third O site, O(3) is bonded in a linear geometry to one Cr(1) and one P(2) atom. In the fourth O site, O(4) is bonded in a bent 120 degrees geometry to one P(1) and one P(2) atom. In the fifth O site, O(5) is bonded in a 3-coordinate geometry to one Li(1), one Cr(1), and one P(1) atom. In the sixth O site, O(6) is bonded in a distorted water-like geometry to one Li(1), one H(4), one H(6), and one H(8) atom. In the seventh O site, O(7) is bonded in a distorted water-like geometry to one Li(2), one H(2), and one H(5) atom. In the eighth O site, O(8) is bonded in a distorted water-like geometry to one Cr(1), one H(6), and one H(7) atom. In the ninth O site, O(9) is bonded in a distorted trigonal planar geometry to one Li(2), one Cr(1), and one P(3) atom. In the tenth O site, O(10) is bonded in a 2-coordinate geometry to one Li(2), one Cr(1), and one P(2) atom. In the eleventh O site, O(11) is bonded in a bent 120 degrees geometry to one P(2) and one P(3) atom. In the twelfth O site, O(12) is bonded in a bent 120 degrees geometry to one P(1) and one P(3) atom. In the thirteenth O site, O(13) is bonded in a 2-coordinate geometry to one P(3) and one H(3) atom. is represented by the CIF card [CIF]
data_LiCrP3H8O13
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   7.185
_cell_length_b   7.693
_cell_length_c   9.965
_cell_angle_alpha   82.722
_cell_angle_beta   74.424
_cell_angle_gamma   77.856
_symmetry_Int_Tables_number   1
_cell_volume   517.249
_cell_formula_units_Z   2
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.000  0.000  0.000  1.0
  Li  Li1  1  0.000  0.500  0.500  1.0
  Cr  Cr2  1  0.807  0.819  0.770  1.0
  Cr  Cr3  1  0.193  0.181  0.230  1.0
  P  P4  1  0.326  0.805  0.742  1.0
  P  P5  1  0.242  0.806  0.475  1.0
  P  P6  1  0.593  0.459  0.731  1.0
  P  P7  1  0.407  0.541  0.269  1.0
  P  P8  1  0.758  0.194  0.525  1.0
  P  P9  1  0.674  0.195  0.258  1.0
  H  H10  1  0.360  0.980  0.964  1.0
  H  H11  1  0.819  0.817  0.430  1.0
  H  H12  1  0.311  0.862  0.101  1.0
  H  H13  1  0.920  0.739  0.205  1.0
  H  H14  1  0.691  0.694  0.398  1.0
  H  H15  1  0.858  0.665  0.009  1.0
  H  H16  1  0.651  0.628  0.001  1.0
  H  H17  1  0.099  0.660  0.086  1.0
  H  H18  1  0.901  0.340  0.914  1.0
  H  H19  1  0.349  0.372  0.999  1.0
  H  H20  1  0.142  0.335  0.991  1.0
  H  H21  1  0.309  0.306  0.602  1.0
  H  H22  1  0.080  0.261  0.795  1.0
  H  H23  1  0.689  0.138  0.899  1.0
  H  H24  1  0.181  0.183  0.570  1.0
  H  H25  1  0.640  0.020  0.036  1.0
  O  O26  1  0.474  0.877  0.791  1.0
  O  O27  1  0.270  0.983  0.058  1.0
  O  O28  1  0.193  0.965  0.379  1.0
  O  O29  1  0.361  0.863  0.575  1.0
  O  O30  1  0.112  0.854  0.813  1.0
  O  O31  1  0.974  0.745  0.101  1.0
  O  O32  1  0.826  0.715  0.379  1.0
  O  O33  1  0.788  0.630  0.943  1.0
  O  O34  1  0.758  0.560  0.672  1.0
  O  O35  1  0.083  0.710  0.559  1.0
  O  O36  1  0.422  0.661  0.389  1.0
  O  O37  1  0.381  0.589  0.746  1.0
  O  O38  1  0.417  0.653  0.134  1.0
  O  O39  1  0.583  0.347  0.866  1.0
  O  O40  1  0.619  0.411  0.254  1.0
  O  O41  1  0.578  0.339  0.611  1.0
  O  O42  1  0.917  0.290  0.441  1.0
  O  O43  1  0.242  0.440  0.328  1.0
  O  O44  1  0.212  0.370  0.057  1.0
  O  O45  1  0.174  0.285  0.621  1.0
  O  O46  1  0.026  0.255  0.899  1.0
  O  O47  1  0.888  0.146  0.187  1.0
  O  O48  1  0.639  0.137  0.425  1.0
  O  O49  1  0.807  0.035  0.621  1.0
  O  O50  1  0.730  0.017  0.942  1.0
  O  O51  1  0.526  0.123  0.209  1.0
[/CIF]
.